104 5.2 Four-Wave Mixing

all FWM measurements presented here have been performed at the low temperature of 25 K and with
an excitation density resulting in merely 10^{17}cm^{−3}excitons. This results in increased dephasing times
which is crucial for making this ultrafast process temporally resolvable at all.

The absorption spectrum recorded for the MAPbI_{3}NPl ensemble at said temperature is shown in
Figure 5.4 a. At 25 K the excitonic peak is well observable next to the continuum onset. Each laser
pulse originating from the OPA is divided into two pulses by a beam splitter. These are the two laser
pulses needed in the degenerate time-integrated FWM experiments. Accordingly, the temporal and
spectral profiles of pulse #1 and #2 are identical. Both exhibit a Gaussian-shaped spectrum when
plotted against photon energy and a FWHM of around 27 meV. Their central wavelength can be
shifted by tuning the OPA. Four different scenarios for the excitation wavelength are represented
inFigure 5.4 b. In case (i) the tails of the exciton peak and the excitation spectrum overlap such
that only the 1s exciton may be excited since the continuum transitions may not be reached by the
excitation wavelength centered at 768 nm. Case (iv), entailing a central wavelength of 715 nm, is the
exact opposite to case (i) in the sense that the excitation spectrum has no overlap with the exciton
transition and exclusively excites free e-h pairs in the continuum. The remaining cases (ii) and (iii) are
located in between both aforementioned scenarios and lead to a simultaneous excitation of exciton
and continuum transitions.

(iv) (iii) (i)

(ii)

FWM0.1

1

FWM0.1

1

FWM0.1

1

FWM0.1

1

400 300

200 100

0

-100 pulse delay time in fs

Figure 5.5: Time-Integrated Four-Wave Mixing on MAPbI_{3}Nanoplatelets.FWM decay curves for
the excitation spectra shown inFigure 5.4for a charge carrier density of 10^{17}cm^{−3}at a temperature of
25 K. The central excitation wavelength set by the OPA has a significant influence on the shape and decay
behavior of the time-integrated FWM signal. Panel (i) shows dephasing of the exciton ensemble only,
whereas (ii) and (iii) additionally involve the continuum states with free e-h pairs such that quantum
beating may be observed. Finally, panel (iv) depicts the dephasing process for free e-h pairs which is too
fast to be temporally resolved by the laser pulses.

Figure 5.5shows that the central excitation wavelength significantly affects the appearance of the FWM
decay curves, i.e., the FWM signal plotted against the pulse delay time𝑡_{delay}between pulses #1 and #2.

The first panel, concerning case (i), shows an exponential decay related to the dephasing of excitons.

This will be analyzed and discussed further in the followingSubsection 5.2.1. When increasing the photon energy of the OPA as to reach a wavelength of 750 nm, i.e., case (ii), the excitation pulse spectrally overlaps slightly with the continuum transitions while still mainly exciting the exciton

106 5.2 Four-Wave Mixing
transition. Compared to case (i) a shoulder appears in the FWM signal which is shown in the second
panel ofFigure 5.5. At an even higher photon energy, i.e., in case (iii), this shoulder turns into a clear
beating behavior of the signal which will be the subject ofSubsection 5.2.2. Finally, the FWM curve
shown in the fourth panel (iv) inFigure 5.5indicates that, even at low temperatures, the dephasing of
free e−h pairs is too fast to perform a reasonable data deconvolution for the purpose of extracting the
dephasing time𝑇_{2}for free e-h pairs.

5.2.1 Dephasing of Excitons

As mentioned above, the first panel inFigure 5.5represents case (i) in which only the 1s exciton is
excited such that the decay of coherence for this energetic transition may be observed. For further
analysis, this graph is plotted again inFigure 5.6 aon a linear scale. A fast initial rise of the FWM signal
is observed and after the signal maximum is reached a slower decay takes place. An estimated decay
time of𝑇_{decay}≈200 fs may be extracted from the exponential decay of this curve. As demonstrated
inEquation 2.52and Equation 2.53this decay time𝑇_{decay} is related to the dephasing time𝑇_{2} via
𝑇_{2} = 𝑔 ⋅ 𝑇_{decay}, with𝑔 = 2for the case of a purely homogeneously broadened transition, whereas
𝑔 = 4applies for the case of inhomogeneous broadening.^{130,144}Without making any assumption, the
Γ_{hom}(25 K)value can be calculated for both scenarios usingEquation 2.40. For an inhomogeneously
broadened sampleΓ_{hom}(25 K) = 1.7 meV is obtained and for an homogeneously broadened sample
Γ_{hom}(25 K) =3.4 meV is obtained. The total broadening has been studied in the previous section and
amounts toΓ_{total}(25 K) =24 meV for the MAPbI_{3}NPls. Obviously,Γ_{total}(25 K) > Γ_{hom}(25 K)for both
examined scenarios andΓ_{total}(25 K)is at least a factor of 7 larger than the homogeneous broadening
Γ_{hom}(25 K). This estimate confirms our previous conjecture that inhomogeneous broadening plays an
important role within the NPl ensemble, especially at low temperatures. Therefore, the recorded FWM
signal may safely be deemed a photon echo and accordingly𝑔 = 4has to be applied, i.e.,𝑇_{2} = 4 ⋅ 𝑇_{decay}.
Moreover, this case legitimates the use ofEquation 2.54in modeling the FWM signal. As it is much
larger as compared to𝑇_{2}, the influence of the lifetime𝑇_{1}is negligible in this formula. However, it
is helpful to consider the pulse length of 115 fs since the theoretical model assumes infinitesimally
short, delta function-like laser pulses. To this end, the fitting function ofEquation 2.54was convoluted
with the respective temporal pulse profile. As shown inFigure 5.6 a, the overall theoretical model
given by the dashed blue line agrees very well with the experimentally obtained curve for the FWM
signal. For case (i), in which excitation occurs at the low energy side of the excitonic peak, it
is likely that less present defect-bound excitons are observed as well (see Figure 5.4). For these
excitons, less scattering — and therefore, a slightly increased dephasing time — may be expected,
possibly explaining why the slope of the experimentally obtained curve inFigure 5.6 ais not explicitly
monoexponential.^{207}Still, the theoretical model allows for extracting an exciton dephasing time of
𝑇_{2}(25 K) = (800±20)fs for the studied MAPbI_{3}NPls. Consequently, the homogeneous broadening
at 25 K may be obtained viaΓ_{hom}(25 K) = 2 ℏ/𝑇_{2}(25 K) = (1.7±0.1)meV, yielding an inhomogeneous
broadening ofΓ_{inhom}= (22±1)meV. Since the latter is temperature-independent, it may be indicated
in the plot ofΓ_{total}(𝑇 )inFigure 5.6 bas a horizontal line. This in turn helps to distinguish between
homogeneous and inhomogeneous broadening for all temperatures. This graphical representation
reveals that inhomogeneous broadening is the main cause for transition broadening at low temperatures
𝑇 < 100 K. At around𝑇 = 150 K homogeneous and inhomogeneous broadening exhibit a similar

400 300

200 100

0

-100 pulse delay time in fs

(i)

FWM signal in a.u.

0.5 1

0

### b a

0 50 100 150 200

temperature in K 80

60 20 40 0

phase transition

Γhom(T)

250 300

Γtotal(T) in meV 100

Γinhom

T_{2} ≈ 800 fs T_{2} ≈ 20 fs

Figure 5.6: Dephasing of the Exciton Ensemble. (a)FWM signal decay curve for the excitation
spectrum given by case (i). As shown inFigure 5.4, only the 1s exciton is excited in this case. Consequently,
the decaying FWM signal (dark red curve) represents the dephasing of the exciton ensemble, thereby
giving access to the dephasing time𝑇_{2}= (800±20)fs. The dashed blue curve represents the respective
theoretical model given byEquation 2.54and agrees well with the experimental data when taking into
account pulse length of 115 fs. (b)Total broadening of the exciton transition versus temperature as
already presented inFigure 5.3 b, but for an extended temperature range. Using the dephasing time
𝑇_{2}= (800±20)fs obtained at 25 K, the homogeneous broadening at this temperature may be calculated, i.e.,
Γ_{hom}(25 K) = 2 ℏ/𝑇_{2}(25 K) = (1.7±0.1)meV. Based thereon, the temperature-independent inhomogeneous
broadening may be extracted viaΓ_{inhom} = Γ_{total}(25 K) − Γ_{hom}(25 K) = (22±1)meV. Consequently, the
homogeneous and inhomogeneous contributions to the total broadening of the excitonic level can be
distinguished for all temperatures.

magnitude and for temperatures above this region homogeneous broadening is the main contributor to the total broadening.

Moreover, usingEquation 2.40, the dephasing time𝑇_{2}may be calculated for the whole temperature
range up to 300 K. The underlying calculation is based on the assumption that the total broadening
Γ_{total}(𝑇 )follows the fitted trend as obtained inFigure 5.3also for𝑇 ≥200 K. This approach predicts
a fast exciton dephasing time𝑇_{2}of only 20 fs for MAPbI_{3}NPls at room temperature, showing that
this process cannot possibly be resolved by the laser pulses of the OPA. This value is far shorter
than the pulse length of the used OPA, implying that the cooling of the sample was a crucial step
in order to resolve the FWM signal at all. Just recently, Jha et al. determined the dephasing time of
excitons in bulk MAPbI_{3}films at room temperature using two-dimensional electronic spectroscopy.^{208}
They obtained a value of 50 fs which is in good agreement with the results of this thesis, especially
considering that bulk LHP films are not identical to LHP NPls.

Finally,Γ_{hom,rest}may be calculated via

Γ_{hom,rest} = Γ_{0}− Γ_{inhom}= Γ_{total}(0 K) − Γ_{inhom}. (5.2)
Therefore, in the investigated MAPbI_{3} NPl sampleΓ_{hom,rest} < 2 meV is obtained at an excitation
density of 10^{17}cm^{−3}. This low value confirms that the excitation density has been chosen reasonably

108 5.2 Four-Wave Mixing and moreover it shows, that the total exciton transition broadening in this LHP NC is dominated by exciton-phonon interactions at higher temperatures.

5.2.2 Quantum Beating

As already demonstrated inFigure 5.5, cases (ii) and (iii), entailing a simultaneous coherent excitation of
excitons and continuum transitions, exhibit no strictly monotonous decay. Rather, a beating behavior
is observed in their FWM signals. Naturally, this is only possible if the spectral width of the excitation
pulse is broad enough to cover both transitions. Such types of excitations are also referred to as
exciton wave packets in which the excited transitions may interfere with each other.^{142}

400 300

200 100

0

-100 pulse delay time in fs

(iii)

FWM signal in a.u.

0.5 1

0

T_{B} = h/E_{B}

Figure 5.7: Quantum Beating in the Four-Wave Mixing Signal. FWM signal decay curve for the
excitation spectrum given by case (iii). As shown inFigure 5.4, the spectrum of the excitation pulse
overlaps with the exciton and the continuum transitions to a similar extent. This results in the generation
of a so-called exciton wave packet in which these transitions are excited simultaneously, leading to a
quantum beating behavior of the FWM signal (red curve). A periodicity of𝑇_{B} = (165±10)fs may be
extracted from the quantum beats. Eventually, the exciton binding energy of the MAPbI_{3}NPls may be
accessed via𝐸_{B}= ℎ/𝑇_{B}. Here, it amounts to(25±2)meV. The dashed blue curve represents a theoretical
model for this behavior which is rooted inEquation 2.55, i.e., it is based on the concept of a three-level
system in which both excited states are superimposed.

In case (iii) as discussed here the central wavelength of the excitation pulse lies at 735 nm, such that the 1s exciton and continuum transition are excited to a similar extent (cf.Figure 5.4). The respective decay of the FWM signal is presented inFigure 5.7. The curve represents a behavior commonly referred to as quantum beating, exhibiting a clear signal drop between the first two peaks. This implies that the excitation pulse originating from the OPA is indeed broad enough to generate an excitonic wave packet. Under this condition, so-called quantum beat spectroscopy (QBS) may be performed in order to gain information on the energy spacing between the excited transitions. As shown inFigure 2.19, the simplified concept of a three-level system may be relied on here, such that one of the two excited states represents the 1s exciton and the other is given by the continuum onset.

Now, the eponymous beating arises from alternating constructive and destructive inference in the
respective polarization components. Based thereon,Equation 2.56determines the relation between
the beating period of the FWM signal and the energy spacing between the excited states which is
actually the exciton binding energy𝐸_{B}within this system. The signal decay for this three-level system
is modeled in accordance withEquation 2.55and represented by a dashed blue line inFigure 5.7. Even
though this approximation neglects higher order excitons and treats the continuum onset as a single
transition, the theoretical model proves to be suitable for approximating the experimentally obtained
FWM signal. The beating time𝑇_{B}, which is defined as the time between the 0 fs delay position and
the first beat after the main peak,^{142}can be obtained from the experimental and theoretical curves
and amounts to(165±10)fs. Consequently, a value of𝐸_{B} = ℎ/𝑇_{B}= (25±2)meV is obtained for the

exciton binding energy, fitting well into the range 2–50 meV of previously reported values for MAPbI_{3}
that relied on different experimental approaches at low temperature.^{53}Since this technique is not
strongly influenced by inhomogeneous broadening effects, QBS is an especially convenient approach
for inhomogeneously broadened materials with low exciton binding energies. Due to the inverse
relation between𝐸_{B}and𝑇_{B}, small values for𝐸_{B}lead to long beating times𝑇_{B}which are easier to
detect given that the FWM signal decays sufficiently slowly. Another advantage of QBS is that the
energy spacing is measured directly as a difference between two transitions, rendering an error-prone
assumption of the absolute continuum onset𝐸_{C}unnecessary.

As explained inSubsection 2.1.3and demonstrated inSubsection 4.1.1, the Elliott model may also be
used to extract exciton binding energies from linear absorption data. However, this is effectively
more practical for cases in which inhomogeneous broadening does not hinder the distinction of
the exciton transition from the continuum states. This has been the case for the strongly quantum
confined CsPbBr_{3}NPls with large exciton binding energies (seeFigure 4.2). Summing up, QBS offers
a promising technique for the calculation of small exciton binding energies𝐸_{B}and supplements the
Elliott model in cases where the excited transitions are difficult to distinguish in linear absorption
spectroscopy due to inhomogeneous broadening.

### Diffusion 6

In the preceding chapters, the recombination dynamics and the dephasing behavior of excitons in LHP NCs
have been studied extensively. Therein, the generation of excitons was driven by external light sources and
the excitons stayed within the LHPs. For the most part, however, conventional semiconductor devices rely
on charge transport between various layers of different materials, also involving injection or extraction of
e-h pairs. Therefore, the topic of exciton diffusion is a crucial one when it comes to the applicability of
LHP NCs in future devices. To date, large electron-hole diffusion lengths of approximately one micrometer
have already been reported for bulk films of MAPbI_{3 – x}Cl_{x}.^{156,158}Here, it shall be studied which diffusion
lengths may be achieved for exciton transport in films of fully inorganic CsPbBr_{3}NCs, i.e., the exciton
diffusion length for CsPbBr_{3}nanocubes and nanowires shall be studied, using two different experimental
approaches.

111

112 6.1 Photoluminescence Mapping